HAL Id: hal-02960051
Submitted on 7 Oct 2020
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
Intergranular corrosion: Comparison between
experiments and cellular automata
Simone Guiso, Dung Di Caprio, Jacques de Lamare, B. Gwinner
To cite this version:
Simone Guiso, Dung Di Caprio, Jacques de Lamare, B. Gwinner. Intergranular corrosion:
Compar-ison between experiments and cellular automata. Corrosion Science, Elsevier, 2020, 177, pp.108953.
Intergranular corrosion: comparison between experiments
and cellular automata
Simone Guisoa,b, Dung di Caprioa, Jacques de Lamareb,∗, Benoît Gwinnerb
aChimie ParisTech, PSL Research University, CNRS, Institut de Recherche de Chimie
Paris (IRCP), F-75005 Paris, France
bDes-Service de la Corrosion et du Comportement des Matériaux dans leur Environnement
(SCCME), CEA, Université Paris-Saclay, F-91191, Gif-sur-Yvette, France
In this paper, a 3D cellular automata approach of intergranular corrosion in pre-sented. A model is proposed, along with experimental results both qualitatively (groove morphology, groove angle distribution) and quantitatively (mass loss, corrosion rate, corrosion front evolution). Simulations have been performed us-ing a new asynchronous algorithm: the choice of the most adequate grid is also discussed. The model investigates the statistical variation of the corrosion front and provides useful information to make predictions on material ageing. Keywords: intergranular corrosion, cellular automata, modelling, material ageing, stainless steel
In France, the PUREX (Plutonium and Uranium Rening by EXtraction) process is used to reprocess spent fuel in a nuclear fuel cycle . The process involves the treatment of the spent fuel in hot and concentrated nitric acid for liquid-liquid extraction of the recoverable material (uranium and plutonium). In some particular conditions, the interaction between the nitric media and the structural stainless steel (SS) may lead to intergranular corrosion (IGC) phenomena [1, 2, 3].
Understanding IGC is therefore crucial. This particular type of corrosion promotes grain detachment and leads to corrosion kinetics larger than expected. IGC study is a challenge that involves both experimental campaigns and simu-lation modelling.
Experimentally, IGC corrosion kinetics is mainly studied using weight-loss (WL) techniques and electrochemical measurements. However, experiments are intrinsically limited in duration and cannot always provide sucient informa-tion to predict material behaviour over long time periods. Modelling can then provide an important support.
The way IGC nds its path along grain boundaries is essential to understand IGC corrosion kinetics and may lead to dierent characteristic morphologies in relation to grain detachment. Thus, on the modelling side, dierent paths have been recently investigated, where focus is on the evolution of the corrosion mor-phology. In brick-wall models , the IGC penetration is described as a function of the probability of choosing a dened path in a "wall structure". Monte-Carlo simulations were performed by Lim et al.  to estimate the average IGC pen-etration depth at precise time steps in comparison with experimental tests. A stochastic reduced order model (SROM) was instead proposed by Sarkar et al.  to quantify the uncertainty on IGC rates. Results demonstrate that this approach is more suitable than MC method for this purpose.
Despite all these achievements, the IGC kinetics is yet to be fully understood. In particular, more investigations should be addressed to the morphology charac-terization of the IGC grooves and to their progression inside the material, which is dicult to access experimentally. A complete description of the phenomenon would be an important tool for the industry in strong need of predictive models for material ageing. The objective of this study is to start lling this gap by presenting a predictive tool for material ageing that includes a ne description of the material morphology evolution. In this paper, the study is focused on "non-sensitized" SS. A 3D stochastic CA model is presented and compared with some experimental tests already published [7, 8].
is presented in Section 2, followed by a description of the experimental tests in Section 3, and of the CA model in Section 4, while results are discussed in Section 5. The conclusive remarks are then presented in Section 6. Tables of symbols, abbreviations and references are provided at the end.
From the experimental point of view, IGC has been studied in terms of WL measures. Specimens are usually exposed to a corrosive solution and extracted at precise time steps [7, 9]. The goal is to obtain information on mass loss and corrosion rate as a function of time.
In parallel, electrochemical tests are also performed to evaluate the risk of IGC. More generally, electrochemical measurements are classically used to character-ize dierent aspects of the SS corrosion. For example, the determination of the pitting potential denes the sensitivity to this type of corrosion , double loop electrochemical potentiokinetic reaction tests inquire about the degree of sen-sitization of the SS , electrochemical impedance spectroscopy experiments give information on the limiting corrosion processes . Among those, linear voltammetry is often performed in the case of IGC to investigate whether the SS remains passive (where the SS dissolves slowly and uniformly) or it is polarized in its transpassive state (where IGC occurs) in its chemical environment (see Figure 1) [13, 14].
In order to resist corrosion, the SSs used for structural material are screened in view of their corrosion resistance, optimized and qualied before their use. In particular, austenitic SSs with low carbon, high chromium and controlled silicon and phosphorus contents are preferred . A stable passive layer protects all these materials so that corrosion, in normal conditions, is slow and uniform. However, too oxidizing conditions (e.g. nitric media containing oxidizing ions at high temperature like Vanadium (V)) may promote the deterioration of this passive layer and generate IGC phenomena. In this case, the cathodic reaction (reduction reaction) is fast and can lead to a shift of the corrosion potential to
Figure 1: Simplied scheme of the dierent electrochemical domains.
the transpassive domain, thus exposing materials to IGC attack, as presented in Figure 1.
Normally, grain boundaries (GB) represent barriers that confer strength to metallic materials. However, in some environmental conditions, they are the main source of weakness and failures. Grain boundary degradation includes corrosion, cracking, embrittlement and fractures. According to literature [7, 16] two cases of IGC can be distinguished.
The rst one includes the "sensitized" SSs, which present a relatively high carbon content. When SSs are subjected to long heat treatments at high tem-peratures (for instance, between 500 and 800◦C), Cr and C species may diuse
through the material and precipitate as chromium carbides (Cr23C6) at grain
boundaries. As chromium slowly diuses from the grain matrix, a poor-in-chromium-content region is generated adjacent to Cr23C6 precipitates. In this
region, the chromium content is not sucient to provide a stable passive lm to protect the SS. As a consequence, the SS is exposed to IGC attack . To prevent these phenomena, dierent countermeasures have been considered. In the industrial eld, for example, titanium (Ti) or niobium (Nb) are added to
the material. Their presence in the matrix promotes the formation of TixCor
NbxCprecipitates and prevents the formation of chromium carbides. Thus, the
material maintains its passive layer - rich in chromium - and IGC attacks are avoided [17, 18].
As an alternative, the carbon content in SS may be reduced in order for it to be lower than 0.03 wt.% . In this case, the carbon is soluble in the austenitic structure and it remains uniformly distributed in the crystal structure. The SS is then called "non-sensitized" and chromium carbides formation is avoided dur-ing high temperature treatments. However, IGC can still occur in some specic conditions. In the context of investigations on the corrosion behavior of a SS in a spent fuel reprocessing plant , experimental tests showed that the ma-terial can still be aected by IGC in presence of highly oxidizing media. The degradation of a non-sensitized SS is characterized by the formation of triangu-lar grooves at grain boundaries (as represented in Figure 2). The progression
Figure 2: Cross section of a "non-sensitized" 310L SS suering IGC .
of the grooves in the material bulk may cause grain detachment with a certain periodicity, as shown in Figure 3.
Figure 3: Scanning Electron Microscope observation of detached grains of a "non-sensitized" 304L SS .
have been recently investigated, among those a promising method is to model IGC phenomena through the cellular automata (CA) approach . It consists of a dynamical system where both space and time are discretized [20, 21]. Each site (named cell) is identied by a state (dened from a nite list of possible states) and its spatial coordinates. The dynamics of the system is then regulated by a list of transition rules, which take into account the interaction between neighbouring cells (generally rst-neighbour cells) .
Recently, dierent studies have been performed within this approach. Lishchuk et al.  improved their previous model  by developing a 3D stochastic CA model. A similar result was obtained by Jahns et al.  who, on the other hand, developed a 2D CA model to study the intergranular oxidation phenomenon. Igarashi et al. [26, 27] also focused their studies on the development of a 2D CA model to study IGC in stainless steels, while Di Caprio et al.  developed a 3D stochastic CA model to study IGC, by improving the previous 2D model .
Gwinner et al. [7, 29] proposed a phenomenological geometrical model to estimate the long-term corrosion rate of "non-sensitized" SS suering IGC. The model assumptions are based on experimental observations: grooves grow sym-metrically along the grain boundaries, groove angles are constant with time
during IGC evolution and the groove depth is nearly homogeneous along the surface. Similar observations were obtained by Beaunier et al. , which pro-posed to describe IGC with two principal parameters:
Vgb which represents the grain boundary dissolution rate
Vs which represents the grain dissolution rate
The dierent approaches are summarized in the following Table 1 and 2, along with their main characteristics.
Table 1: Summary of the dierent IGC models with their main features
Model Approach Results
Brick-wall  2D, probabilistic
Minimum IGC path length as a function of time
Comparison with experimental results
Monte-Carlo  3D, probabilistic
Comparison with experimental results
IGC damage depth as a function of the degree of sensitiveness and of time
SROM  1D, mathematical and probabilistic model
Comparison SROM/Monte-Carlo simula-tions
Eect of the uncertainty in an-odic/cathodic sites on the current density
Eect of the domain length on the current
model [7, 29] 2D/3D, deterministic
Groove angular description
Comparison with experimental results
Table 2: Summary of the dierent CA IGC models with their main features
Reference Approach CA grid / cell
 2D, probabilistic Cubic / cubic 2D: 1216 cells/grain 3D: 448000 cells/grain
Comparison with experimental results
Corrosion depth, path length
 3D, probabilistic Cubic / cubic 3D: 448000 cells/grain
Comparison with experimental results
Corrosion depth, path length
 2D, probabilistic Square / Square Hexagonal grains
Comparison with experimental results (only microstructure)
[26, 27] 2D, probabilistic Square / square Grain size randomly
Comparison with experimental results
Corrosion width and depth, corrosion rate
 3D, probabilistic Cubic / cubic Grain size randomly
Corrosion depth and corrosion rate
 2D, probabilistic
Square / square Various types of grains and spatial distributions
Evolution of the corrosion front as a function of dierent spatial arrange-ments (square, brick-wall, polygonal)
Surface roughness prole Corrosion rate
3. Determination of the experimental corrosion velocities
Figure 4: Schematic representation of the corrosion rates (Vgb and Vs, where
Vgb > Vs), the groove depth (H
), the groove angle (α) and the groove inclina-tion (β) .
Experimental tests were performed by Gwinner et al.  on an AISI 310L stainless steel. It presents a low carbon content and was rstly thermally treated (homogenization treatment and quenching) to avoid precipitate formation that would have brought a type of IGC proper to sensitized SS (see Section 2). The SS was exposed to a solution of nitric acid (HNO3), containing an oxidizing ion
2) at boiling temperature, that was renewed after each corrosion period of
160 h. SS specimens were periodically removed and examined. The experimental equivalent thickness loss (ETLexp, in µm) was evaluated with the following
m(t) ρS 10
where m(t) is the cumulated mass loss (in g) at time t, ρ is the SS density (8 g.cm−3) and S is the initial surface of the polished sample (in cm2) that is
rate CRexpis then dened as CRexp t + ∆t 2
= ETLexp(t + ∆t) − ETLexp(t)
where ∆t is the duration of a corrosion period between two mass loss measure-ments.
Besides the experimental tests, a semi-empirical model was also developed to estimate the long term IGC evolution for the SS . According to this model, a triangular groove is represented as in Figure 4.
The model is based on experimental observations of the mass loss kinetics. According to experimental data, the corrosion rate (Vcorr) linearly evolves from
an initial value to a steady-state condition. The initial value corresponds to the metal dissolution at the initial state (t=0), whose value is Vs. The
steady-state value corresponds to the corrosion rate at which the IGC kinetics is fully controlled by grain dropping: in this case, the corrosion rate is equal to V∗
As discussed in , the transition time from the linear trend to the steady-state condition is estimated (in good agreement with the experimental observations) to be at t = 1.5 D
, where D is the average grain dimension.
Following these assumptions, the corrosion rate (Vcorr) can be expressed as:
t ≤ 1.5 D Vgb∗, Vcorr = 2 3 Vgb∗ D V ∗ gb− Vs t + Vs (3) t ≥ 1.5 D Vgb∗, Vcorr = V ∗ gb (4)
Vs and Vgb∗ are then obtained by tting the rst 4 points of the experimental
corrosion rate kinetics with the linear trend of the semi-empirical model. Vgb is then determined by the following formula:
where β is dened in Figure 4 and averaged over dierent grooves . In , Vs = 92µm/y, Vgb∗ = 1287µm/yand β = 35◦ have been obtained.
4. 3D Cellular automata model
The 3D stochastic CA model will hereafter be presented. The methodol-ogy belongs to the so-called "grey-box" class of approaches as it stands be-tween "black-box" and "white-box" models: the former are phenomenological approaches where the model response is directly related to input data but no interpretation nor mechanistic description is introduced; the latter are based on a detailed understanding of physical laws and processes, but are too complex to be implemented. The CA model presented in this paper adopts a simple stochas-tic mesoscopic level of description. The main features of the model are those who characterize the CA approach: a lattice grid, a list of possible cell states, the corrosion rules. The model is then related to "real" space-time quantities by providing space and time scales. Finally, the construction of the Voronoï diagram, used to model the granular microstructure of the material, is detailed.
4.1. Cell states, corrosion rules and probabilities
The CA model is made of a grid of cells that can acquire three possible chem-ical states: IGN, which represents the grain boundaries, GRN that represents the grains and SOL that denes the corrosive agent.
At each iteration i, CA cells can change their state according to the transition rules. In the case of the corrosion process, IGN and GRN cells change their states to SOL according to two eective probabilities, P0
ign for grain boundaries and
Pgrn0 for grains, as presented in Figure 5. When a SOL cell comes into contact with a GRN cell (or IGN cell), a random number δ is drawn and compared to a probability P0
grn (or Pign0 ) associated to the cell according to the following
equations Pgrn0 = Pgrn Nb Nb,max (6a) Pign0 = Pign Nb Nb,max (6b)
where Pgrn and Pign are the intrinsic corrosion probabilities for the GRN and
IGN cells. The ratio Nb
Figure 5: Schematic representation of the corrosion probabilistic transition rule.
where Nb is the number of SOL cells in contact with the considered GRN (or
IGN) cell and Nb,maxis the maximum possible number of SOL cells in contact
with a single cell. If δ < P0
grn (similarly δ < Pign0 ), the cell will change its state to SOL, i.e. the
cell is "corroded", otherwise it keeps its state (and the cell is not "corroded"). In this CA model at mesoscopic scale, the goal of Eq. (6a) and (6b) is to represent the fact that the more SOL cells surround a GRN (or an IGN) cell, the faster corrosion is. The lifetime of a cell is assumed to be directly proportional to the number of surrounding SOL cells, considering the fact that dissolution is proportional to the surface in contact with the solution. This feature is new in such a type of model.
In order to compare the model to experimental data, the choice of both intrinsic corrosion probabilities Pgrn and Pign is crucial. A preliminary study
of pure grain dissolution is rstly performed to assess the functional relation between probabilities and corrosion velocity in the simulation. A system with a single 3D block of GRN cells surrounded by three layers of SOL cells is adopted. The precise number of SOL layers is in fact immaterial as long as all GRN top plane cells are in contact with at least a SOL cell. In this study, the Pgrn
probability is then varied. Following the results in , a hexagonal close-packed (HCP) grid is chosen for this preliminary study.
Figure 6: Grain dissolution velocity vstat
grn and chemical roughness λ
sta-tionary regime as function of the grain corrosion probability Pgrn.
In Figure 6, the results of the study are presented in terms of corrosion velocity vstat
grn (Pgrn)(expressed as the number of GRN cells dissolved per
itera-tions per cell in the horizontal plane) and chemical roughness λstat(P
grn), as a
function of Pgrn in stationary conditions. The chemical roughness, also known
as rugosity in some domains, is the number of GRN cells in contact with at least one SOL cell, normalized with respect to the horizontal surface of the system. This quantity is of interest because it is directly related to the reactivity of the surface, as it gives information on the kinetics. This contrasts with the standard physical roughness (generally dened as the root mean square of the deviation of the prole with respect to the mean height) that is more a morphological in-formation. Note also that the physical roughness increases as a power law with time; a stationary regime is reached only due to nite size eects which limit the power law. Corrosion velocity and chemical roughness are averaged between the iteration n, which indicates the beginning of the stationary regime, and it-eration N, in such away that N − n is a suciently large number of itit-erations
for the average. Their expressions read as vgrnstat(Pgrn) = 1 NXY Ngrn(n) − Ngrn(N ) N − n (7) λ (Pgrn) = 1 NXY N X i=n Ngrn−sol(i) N − n (8)
where Ngrn(i) is the number of GRN cells that are still present in the system
after i iterations and Ngrn−sol(i)is the number of GRN cells that are in contact
with at least one SOL cell at the iteration i, NXY is the total number of cells
that are present in a horizontal XY -plane.
Figure 6 shows that the velocity is a linear function of Pgrn and that the
chemical roughness remains constant with Pgrn.
Figure 7 shows another characterisation of the surface: the percentage his-togram of the number of SOL neighbours for the GRN cells on the surface. Such information is relevant as the probabilities (Eq. (6a) and (6b)) depend on the number of neighbours to a cell. The statistical distribution of all SOL neighbours is shown to remain identical whatever the value of Pgrn.
Figure 7: Distribution of the number Nbof SOL neighbours to GRN cells during
The results above are important in order to set the relations between sim-ulated and experimental quantities and allow the comparison between the two. The linearity of the corrosion velocity with Pgrn indicates that changing Pgrn
is equivalent to scaling the real time duration of a simulation iteration. This means that, in order to represent a given corrosion rate, one can rst associate a simulation iteration i to a given time duration and then tune the value of Pgrn
to obtain the experimental corrosion rate. However, owing to linearity, there is not one sole choice. The same process can be represented by increasing the duration of an iteration (for instance multiplying it by a given coecient) and correlatively decreasing Pgrn (that is dividing it by the same coecient). Note
that, alternatively, it is possible to choose Pgrn and the iteration time step in
accordance to the corrosion rate. In all cases, the system is the same and the quantity of dissolved material per real time units remains unchanged. If the described system is identical, the chemical roughness and the SOL neighbours distribution remain unchanged, independently of Pgrn: which is indeed what
has been proved in the simulations.
Note that the linearity between corrosion rate and probabilities is not evi-dent, as not all algorithms provide such property. In this paper, this property is a consequence of the asynchronous algorithm (Figure 5), where cell states are updated in the order as they come along during simulations. The standard synchronous algorithm (where all lattice cells updating is performed simulta-neously), that was chosen in , does not exhibit linearity between corrosion velocity and Pgrn for all values. A synchronous algorithm was also used in a
previous IGC study in .
An important consequence of the linearity of the corrosion rate with Pgrn, is
that it is possible to model a given vgrn
velocity ratio using an identical Pgrn
In conclusion, the two CA corrosion probabilities (Pgrn and Pign) are chosen
as follows. To achieve faster simulations, the highest probability is associated to the fastest process. Adopting a smaller value is less ecient as some iterations do not lead to a IGN dissolution event. The IGN corrosion probability Pign
is set equal to 1. Then, Pgrn is set in order to have
ratio equal to the experimental ratio vgrn
vign, which in this case corresponds to
≈ 0.0581 (see 3).
The choice of an appropriate grid is important to best describe the behaviour of a material. The specic kinetics of IGN corrosion is related to the crystal-lographic misorientation of adjacent grains and to the chemical composition of these regions. GB are schematically represented as planes and do not have a preferential spatial orientation. Therefore any realistic model must statisti-cally reproduce GB corrosion velocities, which are isotropic and independent on the planar GB spatial orientation. Dealing with CA approach means that simulations are performed on discrete lattices, which therefore are intrinsically anisotropic. A recent study  aimed at nding the best suited lattice to get as close as possible to an isotropic behaviour. It showed that the HCP grid is the closest to an "isotropic" grid in view of IGC corrosion along grain bound-aries. However, this study was performed using a synchronous algorithm, which has been here substituted by an asynchronous algorithm. The purpose of this section is to investigate whether an identical statement can be valuable with the present asynchronous algorithm.
Figure 8: Schematic 3D view of a planar GB (in blue) dened by its polar and azimuthal angles (θ, ϕ) and its normal ~n .
The isotropy performance of the model (grid and algorithm) is estimated by calculating the relative deviation ε (θ, ϕ) of the simulated IGN corrosion velocity with respect to the theoretical (purely isotropic) case
ε (θ, ϕ) = v z,sim ign − v z,th ign vignz,th (9) where vz,sim
ign is the simulated vertical component of the velocity, v z,th
ign = sin(θ)
is the vertical component of the reference isotropic velocity and (θ, ϕ) are the polar coordinates of the grain boundary, as shown in Figure 8. The corrosion probability is here Pign = 1.
As in the previous case, the HCP grid has been chosen. A top view of the grid is presented in Figure 9. Keep in mind that in this grid each cell has 12 neighbouring cells at equal distance, subdivided as follows: 6 cells in the same horizontal plane, 3 cells in the plane directly above and 3 cells in the plane below. An identical spatial layout is repeated every two horizontal planes (ABAB... structure).
The angular distribution of the velocity in the HCP grid is presented in Fig-ure 10 in terms of δ (θ, ϕ) = ε (θ, ϕ) − ε, where ε is the average of ε (θ, ϕ) over
Figure 9: Schematic representation of the HCP grid, with the representation of the vertical cell stacking.
dierent (θ, ϕ) orientations: θ varies between 10◦and 90◦, and ϕ between 0 and
355◦, each of them every 5◦. Results are averaged over four dierent simulation data generated with four dierent random seeds. For a grain boundary thick-ness of two cells, the average deviation ε is equal to -2.05%, which indicates that simulation velocity is slightly lower than the theoretical one. The stan-dard deviation is around 1.58%. Figure 10 shows that the deviation δ stands within 2%, except for particular angles at θ = 90◦ and ϕ = 0 [90◦], which are
characterized by a higher velocity ("red points" in the Figure). To understand these specicities, the layout of the grain boundaries for these particular angles was investigated in detail. It was found that the velocity increase is caused by a thickness eect, which occurs when the IGN plane is parallel to a grid face. In these geometries, despite an integer grain boundary thickness of two, the grain boundary of the HCP lattice appears to be constituted of a slab with an alternation of two and three cells thickness. In the model, the IGN dissolution probability (Eq. 6b) depends on the number of solution neighbours. A thickness larger than two in these directions causes an increase of the velocity. This eect was investigated by varying the GB slab thickness.
Figure 10: Simulated corrosion velocity results for HCP grid, expressed in terms of δ(θ, ϕ) (in percentage colored scale).
(90◦, 0◦) and (90◦, 30◦). These orientations of the grain boundary correspond to the most extreme cases representing respectively the highest and the lowest velocities with respect to the average. For both orientations, the velocity is an increasing function of thickness. Such an outcome is expected since the probability (Eq. 6b) is an increasing function of the number of neighbours, which is larger when thickness increases. However, the velocity dierence between the two orientations decreases when the thickness increases. This can be understood by the relative dierence in thickness between ϕ = 0◦and ϕ = 30◦that decreases
when the slab thickness increases. Note that results are averaged here over 50 dierent simulations: as a consequence, the error bars are small.
In conclusion, the relative small variations between the simulated and the theoretical velocity seen in Figure 10 for asynchronous algorithm conrm the result that was obtained for the synchronous algorithm in : the HCP grid is then chosen for the comparison with the experimental data.
4.3. Space and time, CA to experiments conversion factors
A summary of the main parameters for the experimental setup and the corresponding CA simulations is presented in Table 3. The grain size within the CA model is set by the number of initial seeds Nseed, independently on the
Figure 11: Simulated corrosion velocity as a function of the grain bound-ary thickness for two congurations: (θ, ϕ) = (90◦, 0◦) in blue and (θ, ϕ) =
(90◦, 30◦)in red. Results are averaged over 50 dierent simulations.
value corresponds to a balance between having, within the simulation box, both suciently large grains and a sucient number of grains in order to describe the corrosion progression in the material. The characteristic dimension of a grain is determined by the number of seeds with the following equation:
Dsim = 3
= 272 (10)
where Nxyz is the total number of cells that are present in the system.
To compare experimental data and simulation results, it is necessary to associate the real space and time scales with CA dimensionless quantities. In the CA approach, these scales correspond respectively to the cell distance and to the duration of one iteration. At this point, two conversion factors need to be introduced.
The rst coecient is a space scaling factor A (in µm/cell), which can be calculated by the ratio between the experimental average grain dimension (in µm)  and the CA average grain dimension (in number of cells). In this case, A = 84
272 ≈ 0.309 µm/cell.
Once the spatial scale is dened, the second coecient is the time scaling factor B (in hour/iteration) that enables to convert the duration of a simulation
Table 3: Comparison between experimental and simulation main parameters.
Parameter Experimental tests  CA simulations Dimension 30 × 20 × 1.5mm3 1280 × 1280 × 1280cells Average grain
lateral dimension 84 µm 272cells Stationary vertical
corrosion velocity 1206 ± 152 µm/y 0.446 ± 0.003cell/iteration Corrosion velocities/ probabilities vgb= 1582.3 ± 187 µm/y, vs= 92 ± 46 µm/y Pign = 1, Pgrn ≈ 0.0581
step into "real" hours. It is calculated as the ratio between the stationary CA corrosion velocity and the experimental one. In this case, B = 8760 × 0.446 × 0.309
1206 ≈ 1.0 hour/iteration, where an extra factor 8760 accounts for the change of time unit from years (used in corrosion velocity) to hours (used in the corrosion experiments). The coecient A is also present because the ratio between experimental velocity and CA velocity involves a spatial ratio, with the space expressed once in µm and once in cells. Note that the specic value for Bequal to 1 is not meaningful; it is a coincidence arisen from the experimental conditions and the chosen units.
4.4. Voronoï tessellation
The material microstructure has been reproduced through a Voronoï dia-gram [32, 33]. It consists of a partitioning of the 3D grid into regions originated by a set of starting points, called seeds. To build the Voronoï diagram, a spher-ical region is progressively grown around each seed along all directions: when two regions meet each other, a border is determined along the mediator plane. Then, each seed keeps growing in all directions until all grid cells become part of a region including a seed or a border. Note that periodic boundary conditions are applied by replicating the entire seed spatial distribution to complete the Voronoï structure at boundaries in all directions. Once the Voronoï tessellation is complete, states are assigned to cells: those which belong to borders assume
the IGN state, the others the GRN state. This construction leads to grain boundaries with a precise two cells thickness, reducing the above-mentioned thickness velocity issue.
The initial grid is then obtained by assigning the SOL state to the three uppermost XY -layers: during dissolution, the solution path is conducted from the top of the grid to the bottom. Note that the top layer grain size distribution is dierent than the one in the bulk because the grains on the surface have been cut. An example of the initial grid is represented in Figure 12.
Figure 12: Representation of the 3D initial grid of IGC model.
4.5. Computational setup
The simulation code has been written in C language, in NVIDIA's CUDA environment, and simulations have been performed using NVIDIA Tesla K80 cards in Dell PowerEdge C4130 servers with Intel Xeon E5-2640 processors. A single simulation run takes from 24 to 48 hours, depending on the values that are given to Pgrnand Pign (the higher the values, the lower the simulation time).
To obtain a reasonable statistics, results are averaged over 50 dierent Voronoï diagrams.
5.1. Preliminary observations on the morphology
Figure 13: Microstructure before corrosion of AISI 310L stainless steel  (left) in comparison with a cut view of the Voronoï microstructure (right).
A comparison between a section of the experimental reference test specimen and a section of the 3D CA model is presented in Figure 13. Both structures of grains are similar, although some dierences can be observed. Some grain boundaries are not clearly visible on the experimental image due to a lower reactivity of these grain boundaries during the metallographic etching process. Some crystal twinning appears on the experimental image, which are not mod-elled by CA. A majority of triple grain boundaries forming 120◦ angles suggests
Figure 14: 3D views (left) and 2D sections for the planes indicated in red (on top) of the system at times t = 400, 800, 1200, 1600, 2000 h. Detached grains
Figure 14 shows 3D perspectives and 2D sections of CA simulations during corrosion at t = 400, 800, 1200, 1600, 2000 h. The groove progression inside the material is visible as well as the consequent grain detachment. Good qualita-tive agreement with experimental observations is found (cf. Figure 2). Some detached grains are presented in Figure 15, in comparison with Figure 3.
Figure 15: 3D view of some detached grains at t=1600 h.
Figure 16 shows the distribution of the α0 angles, the α-projection observed
along some 2D cross sections of the system for both experimental tests and CA simulations. Two "real" times, with the correspondent iterations, have been considered: the rst one, t=641h, in the groove progression regime, while the second one, t=1602h, includes the groove progression and the grain detachment phenomena. CA α0 angle distribution is an average over all α0 angles that are
observed in 2 equally spaced cross sections for 10 dierent simulations. In each section, 7 to 8 grooves were generally found.
Results conrm that, in both approaches, the distribution does not have a sig-nicant evolution in time. In the simulations, a narrow peak was found between 5◦ and 15◦, similar to the experimental observations . A comparison of the
main results is presented in Table 4: the dierence between experimental and CA average values of α0 is within the standard deviation. A distribution tail
Figure 16: Comparison of experimental (in pink and red) and CA simulated (light-blue and blue) histogram distributions of groove angles at dierent time steps, t=641 h and t=1602 h, and at corresponding CA iterations. For each set of bars, α0 values are referred to the α0 interval dened by the values in the
abscissa inside which they are represented.
2D sections and are therefore larger than the corresponding α 3D angles, as discussed in .
Table 4: Comparison between experiments and simulations in terms of average alpha and standard deviation at two dierent time steps
Parameter Experimental tests  CA simulations t= 641 h t = 1602 h i = 641 i = 1602 Average alpha 11.6◦ 11.5◦ 10.9◦ 9.9◦
Standard deviation 6.2◦ 5.1◦ 3.8◦ 3.6◦
5.2. Mass loss kinetics
Figure 17 shows the comparison between simulations and experiments, in terms of ETL and CR. CA simulation results have been scaled with the above-mentioned space and time factors. The equivalent thickness loss has been
di-vided in two components: the ETL due to the material dissolution (represented in black) and the one due to grain dropping (dierence between the red squared points and the black curve). This distinction is not possible in the experiments. In order to match the denitions that were used in , the following corre-sponding denitions are considered
Nmat(0) − Nmat(t)
where Nmat(t)is the sum of the number of IGN and GRN cells at time t, NXY
is the number of grid cells in a XY -plane and A is the space scaling factor. Note that, as the horizontal axis are now plotted in real time, iteration i can be replaced with time t, as B = 1.
The corrosion rate is dened by
t + ∆t
= ETLsim(t + ∆t) − ETLsim(t)
B (12) where ∆t is chosen equal to 160 (a time interval large enough to average corro-sion rates), the factor 8760 is introduced again to have standard corrocorro-sion rates in µm/y.
Figure 17: Weight loss comparison between CA simulations (in red) and ex-perimental tests (in blue). The black line represents the portion of equivalent thickness loss that comes from the material dissolution.
The 3D CA model shows a good agreement with the experimental tests. At the beginning, the corrosion rate grows linearly with time while the equivalent
thickness loss squarely evolves with it. Then, a transition regime is observed between 600 h and 1000 h. After t=1000 h, the corrosion rate becomes constant and the weight loss increases linearly with time. This behaviour is related to the morphology of the system. Firstly, grooves are formed and progress into the material, causing a progressive grain detachment. Then, grains start dropping with a certain periodicity (depending on the size). On average, when the rst grain layer is detached, a stationary corrosion rate is reached.
5.3. Evolution of the surface morphology
The considerations on the mass loss discussed in the previous paragraph give only a mean information of the degradation of the SS in terms of mean thickness loss. However, taking into account the localized character of IGC, the corrosion is deeper in some locations of the SS like at the bottom of the grooves, as illustrated in Figure 2 and Figure 14. As these points dene the residual available thickness of SS, it is fundamental to have information on their time-dependent position. However, information on the deepest corrosion is experimentally only accessible through analysis of 2D cross sections (Figure 2) which destroy the material.
Figure 18: Comparison of the relative surface with experimental results in blue and simulated results in red. The error bars are estimated at 2σ/√Z, where σ is the standard deviation and Z is the number of tests.
The evolution of the relative corrosion surface gives a rst set of information on this aspect. It is dened as the ratio of the corroded surface at time t to the corresponding initial planar surface. In practice it can be calculated from 2D cross section pictures, as the ratio of the contours of the corroded surface to their horizontal projection. A comparison between numerical and experimental results is given in Fig. 18. The numerical results were obtained by averaging over four equally spaced cross sections and ten Voronoï structures.
Both curves present a similar trend. The relative surface evolution starts with a transitory regime up to around t=500 h; then the stationary regime starts. Once again, the trend of this parameter reects the two corrosion regimes: groove progression (transitory) and grain detachment (stationary). CA results are comparable with experimental ones. The dierences between the two curves is within the error bars.
5.4. Evolution of the distribution of the deepest penetrations
Figure 19: Representation of the grain boundary - solution interface during corrosion.
At a given corrosion time, the spatial distribution of the deepest points of the grooves corresponds to the spatial distribution of the grain boundary cells that are in contact with the solution (IGN-SOL). An example of an IGN-SOL interface is presented in Figure 19. It should be noted that the synchronous algorithm adopted in  for Pign = 1showed a homogeneous dissolution of IGN
is more satisfactory in this case, since it shows a distribution of such points similar to experimental observations.
Figure 20: IGN-SOL spatial distribution as a function of the depth for experi-mental results (red shades) et CA simulations (blue shades). Lines are provided as guides.
The IGN-SOL spatial distribution has been calculated every 25 simulation steps for the dierent Voronoï structures. The distributions present a Gaussian-type pattern, as shown in Figure 20. It diers slightly from a perfect "bell curve" since the corrosion algorithm involves non-independent events. The two approaches show the same trend, although their denition is slightly dierent. CA simulations consider, at each (x,y) coordinate, the lowest IGN cell that is in contact with a SOL cell, while experiments consider only the lowest points of the grain boundary grooves. At low depth, a narrow peak is present; then, as the depth increases, the number of non-independent events increases and the distribution spreads. When the rst grain characteristic dimension is reached on average in terms of depth and grain detachment starts, a small hump appears aside the main distribution peak.
The evolution of the IGN-SOL interface depth as a function of time is pre-sented in Figure 21. The three curves represent respectively the minimum (in red), the average (in blue) and the maximum (in black) depths, estimated every 25 simulations (which correspond to 25 hours). The average and the maximum
Figure 21: Representation of the average IGN-SOL interface depth as a function of time. Results are calculated every 25 simulation steps.
interface depths present a linear trend. The minimum interface depth presents instead a linear trend up to 500 h, then it switches to another linear trend with a slightly higher slope. This particular behaviour is again linked to the two regimes that characterize the IGC phenomenon. These data have a high indus-trial interest, since they give important information on when a material may reach a critical failure point in terms of corrosion.
Figure 22: Representation of the standard deviation of the IGN-SOL spatial distribution as a function of time.
depth distribution is shown in Figure 22. At rst, it seems to follow a linear trend; then it switches to a square-root-of-time trend. The two trends corre-spond to the two morphological regimes that characterize the IGC, as seen in Figure 20. The linear regime matches with the groove progression inside the material, while the second one reects the combination of the previous eect together with grain detachment. Due to the limited dimensions of the simulated systems, the grain detachment events have a large impact on the corrosion pro-gression and explain the oscillations at t > 1000 h.
CA modelling has been used as a so called grey box approach. Like for all simulations, it is necessary to introduce in the simulation the real space and time scales. For the space, the relation between grain size and number of cells is chosen. There is no unique choice: a "best choice" is made to suciently balance a detailed description (large lattice) and the simulation time (not too large lattice). The time scale is then derived from a velocity ratio using the sta-tionary IGC velocity as reliable physical quantity, as it is obtained as an average over several points. Finally, the grain corrosion velocity is taken from the ex-perimental study. It should be noted that, as a grey box approach, the method cannot predict corrosion rates, but it uses coecients provided experimentally. However, by only using three input numbers (two of them (A and B) are necessary to give a meaning to the simulation) several results (in the form of trends or graphs) are obtained. The main results are listed below.
The model reproduces several IGC features that are compared to experi-mental results of :
the Voronoï tessellation reasonably accounts for the material mor-phology;
the approach shows the characteristic grooves expected for "non-sensitized" SS IGC corrosion;
the ETL and corrosion velocity curves are well reproduced and ex-hibit the two characteristic corrosion kinetic regimes;
the relative surface morphology is also reproduced.
New features are obtained:
information about grain dropping and pure granular dissolution have been separated;
lowest corrosion point depth distribution histogram is traced; supplementary information of minimum and maximum of these points
and their standard deviation have been obtained.
Note that some features are dicult to obtain experimentally as they concern the bulk material and require the physical destruction of the sample as they cannot be performed in situ.
In this paper, a 3D cellular automata model is proposed to investigate the IGC phenomenon. The model provides realistic morphological characteristics of IGC like groove shaped corrosion, grain detachment. The model can be consid-ered as a grey box approach. The approach feeds on experimental parameters and combines them with mechanistic features within the CA approach. Here, corrosion velocities are used to parametrize the corrosion probabilities of the model. In contrast with [19, 31], a new asynchronous algorithm has been used which ensures linearity between CA parameters and real corrosion kinetics. This is useful to treat IGC modelling which involves dierent corrosion kinetics for granular and intergranular material.
Concerning the quantitative comparison, a particular attention has been spent to validate the choice of the CA grid. The model can thus provide quantita-tive kinetics of the ETL and angular distribution of the grooves. The model also gives new insights on IGC as it is able to separate the contributions from granular and intergranular corrosion and gives the statistical spatial distribu-tion of the penetradistribu-tion depths of the corrosion. The precise knowledge of this distribution is of critical interest for managing intergranular corrosion of SS in industry. These features help characterizing the material dissolution and assess system reliability predictions.
This article shows how to pass from experimental to simulation quantities. The model is simple and draws input parameters directly from phenomenological corrosion velocities. However, ner mechanistic descriptions can be considered in the future. For instance, the corrosion probabilities can be based on intrinsic quantities like energetic barriers and allow taking into account temperature eects. A detailed description of the environment can also be examined. In this model, a simplied eect of the strength of the solution is introduced by connecting the corrosion probability to the amount of solution surrounding a corroded cell. In the future, it will also be possible to account for diusion and concentration eects of corrosive compounds in solution.
The authors would like to thank Damien Féron for his useful comments on this paper, and the CEA and the National Graduate School of Chemistry in Paris for supporting this work.
The raw/processed data required to reproduce these ndings cannot be shared at this time as the data also form part of an ongoing study.
Table 5: List of symbols
t, ∆t time, time duration in experiments in hours h i, ∆i iteration, number of iterations in the simulation
m(t) experimental cumulated mass loss as a function of t in g ρ SS density in g.cm−3
S initial surface of polished sample in cm2
Dexp, Dsim characteristic size of grains for experiments in µm and for simulations in number
ETLexp(t), ETLsim(i) equivalent thickness loss as a function of time t for experiments and iterations
CRexp(t), CRsim(i) corrosion velocity as a function of time t for experiments and iterations i for
vign(t), vign(i) grain boundary corrosion rate (corresponding to Vgb in article ) as a function
of time t for experiments and iterations i for simulations
vgrn(t), vgrn(i) grain corrosion rate (Vs in article ) as a function of time t for experiments
and iterations i for simulations α, β groove angles see Figure 4 in degrees◦ H0∗ groove depth see Figure 4
NX, NY, NZ dimensions of the system in the CA simulations in number of cells
Nb number of SOL neighbours to a cell
Nb,max maximum number of neighbours to a cell, 12 for HCP lattice
Pgrn corrosion probability for grain corrosion
Pign corrosion probability for intergranular corrosion
grn(Pgrn) stationary corrosion velocity of grains as a function of grain corrosion probability
λstat(Pgrn) stationary chemical roughness as a function of grain corrosion probability
Ngrn number of grain cells (GRN) in the system
Nmat number of grain (GRN) and intergranular (IGN) cells in the system
Ngrn−sol number of grain cells in contact with at least a SOL cell
Table 6: List of abbreviations
PUREX: Plutonium and Uranium Rening by Extraction IGC: intergranular corrosion
SROM: stochastic reduced order model SS: stainless steel
AISI: American Iron and Steel Institute GB: grain boundaries
HCP: hexagonal close-packed grid CA: cellular automata
Cellular automata type of cells: SOL solution, GRN grain, IGN intergranular cells
CUDA: Compute Unied Device Architecture
 P. Fauvet, Corrosion issues in nuclear fuel reprocessing plants, Elsevier Ltd, 2012. doi:10.1533/9780857095343.5.679.
 G. Andreoletti, P. Chambrette, A. Mercier, J.-P. Moulin, F. Thurin, C. Vit-toz, Industrial feedback of intercycle uranyl nitrate concentration in stain-less steel 304L evaporator, Eurocorr 2006, Maastricht, the Netherland (2006).
 F. Ueno, C. Kato, T. Motooka, S. Ichikaway, M. Yamamoto, Corrosion phenomenon of stainless steel in boiling nitric acid solution using large-scale mock-up of reduced pressurized evaporator, Journal of Nuclear Sci-ence and Technology 45 (10) (2008) 10911097. doi:10.1080/18811248. 2008.9711897.
IGC growth in aluminum alloys, Journal of Statistical Planning and Infer-ence 137 (7) (2007) 24052412. doi:10.1016/j.jspi.2006.09.021.  M. L. C. Lim, R. G. Kelly, J. R. Scully, Overview of intergranular
corro-sion mechanisms, phenomenological observations, and modeling of AA5083, Corrosion 72 (2) (2016) 198220. doi:10.5006/1818.
 S. Sarkar, J. E. Warner, W. Aquino, M. D. Grigoriu, Stochastic reduced order models for uncertainty quantication of intergranular corrosion rates, Corrosion Science 80 (2014) 257268. doi:10.1016/j.corsci.2013.11. 032.
 B. Gwinner, M. Auroy, F. Balbaud-Célérier, P. Fauvet, N. Larabi-Gruet, P. Laghoutaris, R. Robin, Towards a reliable determination of the inter-granular corrosion rate of austenitic stainless steel in oxidizing media, Cor-rosion Science 107 (2016) 6075. doi:10.1016/j.corsci.2016.02.020.  E. Tcharkhtchi-Gillard, M. Benoit, P. Clavier, B. Gwinner, F. Miserque,
V. Vivier, Kinetics of the oxidation of stainless steel in hot and concentrated nitric acid in the passive and transpassive domains, Corrosion Science 107 (2016) 182192. doi:10.1016/j.corsci.2016.02.031.
 G. O. H. Whillock, B. F. Dunnett, Intergranular corrosion testing of austenitic stainless steels in nitric acid solutions, presented at the Euro-corr 2004, Société de Chimie Industrielle, Paris (France) (2004) 110.  Standard Test Method for Conducting Cyclic Potentiodynamic Polarization
Measurements for Localized Corrosion Susceptibility of Iron-, Nickel-, or Cobalt-Based Alloys, ASTM G61 (2018).
 Standard Test Method for Electrochemical Reactivation (EPR) for Detect-ing Sensitization of AISI Type 304 and 304L Stainless Steels, ASTM G108 (2015).
 M. Orazem, B. Tribollet, Electrochemical Impedance Spectroscopy, 2nd Edition, Wiley-Interscience, 2017.
 S. Ningshen, M. Sakairi, Corrosion degradation of AISI type 304l stainless steel for application in nuclear reprocessing plant, Journal of Solid State Electrochemistry 19 (12) (2015) 35333542. doi:10.1007/ s10008-015-2891-y.
 E. F. Diaz, C. Cuevas-Arteaga, N. Flores-García, S. Mejía Sintillo, O. Sotelo-Mazón, Corrosion performance of AISI-309 exposed to molten salts V2O5- Na2SO4at 700◦C applying EIS and R p electrochemical
tech-niques, Journal of Spectroscopy 2015 (2015) 112. doi:10.1155/2015/ 826759.
 J. S. Armijo, Intergranular corrosion of nonsensitized austenitic stainless steels, Corrosion 24 (1968) 2430.
 W. D. Callister, Materials science and engineering: an introduction, 7th Edition, John Wiley & Sons, 2007.
 C. Singh, H. Kumar, R. Kumar, Research on the diusion of ti-based sta-bilizer through ux coated GTAW to reduce carbide precipitation in SS304 weldment, Materials Today: Proceedings 5 (9) (2018) 1868918696.
 K. E. Pinnow, A. Moskowitz, Corrosion resistance of stainless steel weld-ments, Weld J. 49 (6) (1970) 278284.
 D. di Caprio, J. Staej, G. Luciano, L. Arurault, 3D cellular automata sim-ulations of intra and intergranular corrosion, Corrosion Science 112 (2016) 438450. doi:10.1016/j.corsci.2016.07.028.
 C. F. Pérez-Brokate, D. di Caprio, E. Mahé, D. Féron, J. de Lamare, Cyclic voltammetry simulations with cellular automata, Journal of Computational Science 11 (2015) 269278. doi:10.1016/j.jocs.2015.08.005.
 B. Chopard, M. Droz, Cellular Automata Modeling of Physical Systems, Cambridge University Press, 1998.
 P. Cordoba-Torres, K. Bar-Eli, V. Fairen, Non-diusive spatial segregation of surface reactants in corrosion simulations, Journal of Electroanalytical Chemistry 571 (2) (2004) 189200. doi:10.1016/j.jelechem.2004.05. 009.
 S. Lishchuk, R. Akid, K. Worden, J. Michalski, A cellular automaton model for predicting intergranular corrosion, Corrosion Science 53 (2011) 2518 2526. doi:10.1016/j.corsci.2011.04.027.
 S. Lishchuk, R. Akid, K. Worden, Model-based prognosis for intergranular corrosion, in: Proceedings of the 4th European Workshop on Structural Health Monitoring, 2008, pp. 340348.
 K. Jahns, K. Balinski, M. Landwehr, V. B. Trindade, J. Wubbelmann, U. Krupp, Modeling of intergranular oxidation by the cellular automata approach, Oxidation of Metals 87 (3) (2017) 285295. doi:10.1007/ s11085-017-9732-6.
 T. Igarashi, A. Komatsu, T. Motooka, F. Ueno, Y. Kaji, M. Yamamoto, Simulations of intergranular corrosion feature for stainless steel using cel-lular automata method, Zairyo to Kankyo/ Corrosion Engineering 63 (7) (2014) 431437. doi:10.3323/jcorr.63.431.
 F. Ueno, A. Komatsu, T. Igarashi, M. Yamamoto, Study of the eect of phosphorus concentration on intergranular corrosion of stainless steel in boiling nitric acid solution, in: Eurocorr Pisa (Italy), 2014.
 A. Taleb, J. Staej, Numerical simulation of the eect of grain size on corrosion processes: Surface roughness oscillation and cluster detachment, Corrosion Science 53 (8) (2011-08) 25082513. doi:10.1016/j.corsci. 2011.04.008.
 B. Gwinner, J.-M. Borgard, E. Dumonteil, A. Zoia, A stereological ap-proach for measuring the groove angles of intergranular corrosion, Corro-sion Science 115 (2017) 17. doi:10.1016/j.corsci.2016.11.005.
 L. Beaunier, M. Froment, C. Vignaud, A kinetical model for the electro-chemical grooving of grain boundaries, Electrochimica Acta 25 (10) (1980) 12391246.
 S. Guiso, D. di Caprio, J. de Lamare, B. Gwinner, Inuence of the grid cell geometry on 3D cellular automata behavior in intergranular corrosion, Submitted to Journal of Computational Science.
 A. Okabe, A. Suzuki, Locational optimization problems solved through voronoi diagrams, European Journal of Operational Research 98 (3) (1997) 445456. doi:10.1016/S0377-2217(97)80001-X.
 G. Voronoi, Nouvelles applications des paramètres continus la théorie des formes quadratiques. deuxième mémoire, recherches sur les parallélloèdres primitifs", Journal für die Reine und Angewandte Mathematik 134 (1908) 198287.